#------------------------------------------------------------------------------
#$Date: 2017-11-04 04:03:29 +0200 (Sat, 04 Nov 2017) $
#$Revision: 202575 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/51/42/4514278.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4514278
loop_
_publ_author_name
'Zhao, Min'
'Zhang, Xian-Wei'
'Wu, Chuan-De'
_publ_section_title
;
 Structural Transformation of Porous Polyoxometalate Frameworks and Highly
 Efficient Biomimetic Aerobic Oxidation of Aliphatic Alcohols
;
_journal_issue                   10
_journal_name_full               'ACS Catalysis'
_journal_page_first              6573
_journal_paper_doi               10.1021/acscatal.7b01985
_journal_volume                  7
_journal_year                    2017
_chemical_formula_sum            'Cu2 Gd4 H104 O120 W19 Zn3'
_chemical_formula_weight         6470.17
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                91.749(2)
_cell_angle_beta                 101.863(2)
_cell_angle_gamma                113.393(2)
_cell_formula_units_Z            2
_cell_length_a                   16.3885(3)
_cell_length_b                   16.5970(3)
_cell_length_c                   21.2038(5)
_cell_measurement_reflns_used    84367
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.37
_cell_measurement_theta_min      2.75
_cell_volume                     5139.8(2)
_computing_cell_refinement       'CrysAlisPro (Oxford Diffraction Ltd., 2010)'
_computing_data_collection       'CrysAlisPro (Oxford Diffraction Ltd., 2010)'
_computing_data_reduction        'CrysAlisPro (Oxford Diffraction Ltd., 2010)'
_computing_molecular_graphics    'Diamond 3.1a (Brandenburg, 2005)'
_computing_publication_material  'PLATON (Spek, 2009)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.3592
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini ultra'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0670
_diffrn_reflns_av_sigmaI/netI    0.0595
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            84367
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         2.75
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    24.923
_exptl_absorpt_correction_T_max  0.106
_exptl_absorpt_correction_T_min  0.039
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   CrysAlisPro
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    4.181
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             5748
_exptl_crystal_size_max          0.46
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.09
_refine_diff_density_max         3.101
_refine_diff_density_min         -2.781
_refine_diff_density_rms         0.365
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1363
_refine_ls_number_reflns         20996
_refine_ls_number_restraints     18
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0651
_refine_ls_R_factor_gt           0.0426
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0415P)²+34.4070P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0924
_refine_ls_wR_factor_ref         0.1032
_reflns_number_gt                15914
_reflns_number_total             20996
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cs7b01985_si_002.cif
_cod_data_source_block           CZJ-11
_cod_original_cell_volume        5139.77(18)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4514278
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W1 W 1.41776(3) 0.93756(4) -0.19251(3) 0.01859(12) Uani 1 1 d .
W2 W 0.64236(4) 0.63530(4) -0.14257(3) 0.02065(12) Uani 1 1 d .
W3 W 0.73845(4) 0.79390(3) -0.32819(3) 0.01882(12) Uani 1 1 d .
W4 W 0.76599(3) 0.63440(3) -0.39703(2) 0.01778(12) Uani 1 1 d .
W5 W 1.28166(4) 0.72950(4) -0.19341(3) 0.01972(12) Uani 1 1 d .
W6 W 0.78125(4) 0.84391(4) -0.15031(3) 0.01996(12) Uani 1 1 d .
W7 W 1.36508(4) 0.90002(4) -0.37305(3) 0.01943(12) Uani 1 1 d .
W8 W 0.68076(4) 0.45317(4) -0.21796(3) 0.02189(13) Uani 1 1 d .
W9 W 1.25140(4) 0.88774(4) -0.11882(2) 0.01865(12) Uani 1 1 d .
W10 W 0.84826(4) 0.49226(3) -0.28986(3) 0.01931(12) Uani 1 1 d .
W11 W 1.11639(4) 0.99966(4) -0.37084(3) 0.02280(13) Uani 1 1 d .
W12 W 1.33178(4) 1.08448(4) -0.28809(3) 0.02221(13) Uani 1 1 d .
W13 W 0.59407(3) 0.58826(4) -0.32509(3) 0.01870(12) Uani 1 1 d .
W14 W 0.85937(4) 0.72804(4) -0.05885(3) 0.02323(13) Uani 1 1 d .
W15 W 1.21764(4) 0.69414(4) -0.37658(3) 0.02049(12) Uani 1 1 d .
W16 W 1.16397(4) 1.03652(4) -0.21327(3) 0.02046(12) Uani 1 1 d .
W17 W 1.04300(4) 0.70255(4) -0.21389(3) 0.02212(13) Uani 1 1 d .
W18 W 1.14932(4) 0.82599(4) -0.45870(3) 0.02368(13) Uani 1 1 d .
W19 W 0.89074(4) 0.53507(4) -0.13193(3) 0.02142(12) Uani 1 1 d .
Gd1 Gd 0.63430(5) 0.97207(5) -0.37684(3) 0.02560(16) Uani 1 1 d .
Gd2 Gd 1.32234(4) 0.51691(4) -0.42409(3) 0.02026(15) Uani 1 1 d .
Gd3 Gd 0.87700(6) 0.63819(6) 0.11803(4) 0.0380(2) Uani 1 1 d .
Gd4 Gd 1.32066(4) 0.99639(4) 0.07453(3) 0.01993(15) Uani 1 1 d .
Zn1 Zn 0.82878(10) 0.68068(9) -0.22438(7) 0.0157(3) Uani 1 1 d .
Zn2 Zn 1.18429(10) 0.85312(9) -0.28874(7) 0.0158(3) Uani 1 1 d .
Zn3 Zn 0.97132(9) 0.82547(9) -0.29841(6) 0.0117(3) Uani 1 1 d .
Cu1 Cu 1.01038(10) 0.86406(10) -0.14792(7) 0.0177(3) Uani 1 1 d .
Cu2 Cu 0.99846(10) 0.67508(10) -0.37129(7) 0.0176(3) Uani 1 1 d .
O1 O 1.0203(6) 0.9054(7) -0.3605(4) 0.028(2) Uani 1 1 d .
O2 O 0.9959(6) 0.6407(6) -0.1494(4) 0.023(2) Uani 1 1 d .
O3 O 0.7262(6) 0.8163(5) -0.2422(4) 0.020(2) Uani 1 1 d .
O4 O 1.3823(6) 0.9475(6) -0.1114(4) 0.025(2) Uani 1 1 d .
O5 O 1.2010(6) 0.9744(6) -0.2873(4) 0.020(2) Uani 1 1 d .
O6 O 0.7457(5) 0.6723(5) -0.3061(4) 0.0141(18) Uani 1 1 d .
O7 O 1.2251(6) 0.8247(6) -0.3622(4) 0.020(2) Uani 1 1 d .
O8 O 0.7369(6) 0.7335(6) -0.4108(4) 0.0193(19) Uani 1 1 d .
O9 O 1.0590(6) 0.7678(6) -0.2931(4) 0.019(2) Uani 1 1 d .
O10 O 1.5346(6) 0.9804(6) -0.1584(5) 0.029(2) Uani 1 1 d .
O11 O 0.6316(6) 0.5613(6) -0.3975(4) 0.020(2) Uani 1 1 d .
O12 O 1.1064(6) 0.6466(6) -0.3635(4) 0.026(2) Uani 1 1 d .
O13 O 0.8611(6) 0.8472(6) -0.3079(4) 0.021(2) Uani 1 1 d .
O14 O 1.1417(6) 0.6802(6) -0.2141(4) 0.021(2) Uani 1 1 d .
O15 O 0.7476(7) 0.9290(6) -0.1311(4) 0.026(2) Uani 1 1 d .
O16 O 0.6227(6) 0.4880(5) -0.2896(4) 0.023(2) Uani 1 1 d .
O17 O 0.5390(6) 0.5839(7) -0.1225(5) 0.029(2) Uani 1 1 d .
O18 O 1.3477(6) 0.7812(6) -0.3817(4) 0.0185(19) Uani 1 1 d .
O19 O 1.2660(6) 0.7750(5) -0.1136(4) 0.020(2) Uani 1 1 d .
O20 O 0.9634(6) 0.7896(6) -0.0811(4) 0.026(2) Uani 1 1 d .
O21 O 0.6036(6) 0.7005(6) -0.3457(4) 0.022(2) Uani 1 1 d .
O22 O 1.2921(7) 1.1213(6) -0.2200(5) 0.030(2) Uani 1 1 d .
O23 O 1.2939(6) 0.6370(6) -0.1678(5) 0.028(2) Uani 1 1 d .
O24 O 1.0423(7) 0.7662(7) -0.4444(5) 0.032(2) Uani 1 1 d .
O25 O 1.2577(6) 0.9102(6) -0.0374(4) 0.021(2) Uani 1 1 d .
O26 O 0.5964(7) 0.3517(6) -0.2145(5) 0.033(2) Uani 1 1 d .
O27 O 1.4270(7) 1.1811(6) -0.2883(5) 0.033(2) Uani 1 1 d .
O28 O 0.7758(6) 0.4426(6) -0.1435(5) 0.027(2) Uani 1 1 d .
O29 O 0.7060(6) 0.8727(6) -0.3642(4) 0.022(2) Uani 1 1 d .
O30 O 0.8792(7) 0.4267(7) -0.3349(5) 0.034(3) Uani 1 1 d .
O31 O 0.7855(6) 0.7183(5) -0.1561(4) 0.0171(19) Uani 1 1 d .
O32 O 0.9548(6) 0.7626(6) -0.2191(4) 0.0190(19) Uani 1 1 d .
O33 O 0.8097(6) 0.5581(6) -0.2184(4) 0.020(2) Uani 1 1 d .
O34 O 1.3975(6) 1.0354(6) -0.2151(4) 0.026(2) Uiso 1 1 d .
O35 O 0.6055(6) 0.6231(6) -0.2359(4) 0.025(2) Uani 1 1 d .
O36 O 1.2402(6) 0.6049(6) -0.3985(4) 0.023(2) Uani 1 1 d .
O37 O 0.8229(6) 0.8262(6) -0.0599(4) 0.027(2) Uani 1 1 d .
O38 O 0.7472(6) 0.5927(6) -0.4774(4) 0.022(2) Uani 1 1 d .
O39 O 1.2724(6) 0.8543(6) -0.2110(4) 0.0191(19) Uani 1 1 d .
O40 O 1.4258(6) 0.6696(6) -0.3982(4) 0.026(2) Uani 1 1 d .
O41 O 0.7866(6) 0.5368(6) -0.3539(4) 0.021(2) Uani 1 1 d .
O42 O 0.9527(7) 0.5040(7) -0.0705(5) 0.031(2) Uani 1 1 d .
O43 O 1.2315(6) 0.9820(6) -0.1523(4) 0.022(2) Uani 1 1 d .
O44 O 1.2694(6) 0.7092(6) -0.2828(4) 0.022(2) Uani 1 1 d .
O45 O 0.7245(6) 0.6514(6) -0.0616(4) 0.024(2) Uani 1 1 d .
O46 O 1.1795(7) 0.7234(6) -0.4633(4) 0.028(2) Uani 1 1 d .
O47 O 1.0639(7) 0.9396(6) -0.2135(5) 0.030(2) Uani 1 1 d .
O48 O 0.7375(6) 0.4064(6) -0.2761(4) 0.026(2) Uani 1 1 d .
O49 O 0.8920(6) 0.9009(6) -0.1611(5) 0.027(2) Uani 1 1 d .
O50 O 1.1247(6) 0.8113(6) -0.1547(4) 0.025(2) Uani 1 1 d .
O51 O 1.3517(6) 1.0037(6) -0.3430(4) 0.024(2) Uani 1 1 d .
O52 O 0.9140(6) 0.4793(6) -0.2034(4) 0.026(2) Uani 1 1 d .
O53 O 1.3220(7) 0.3761(7) -0.3952(5) 0.038(3) Uani 1 1 d .
O54 O 1.4328(7) 0.5412(7) -0.4873(5) 0.033(3) Uani 1 1 d .
O55 O 1.2613(7) 1.0814(7) -0.0044(4) 0.033(2) Uani 1 1 d .
O56 O 1.4041(6) 0.8112(6) -0.1749(4) 0.023(2) Uani 1 1 d .
O57 O 0.6645(6) 0.5274(6) -0.1601(5) 0.027(2) Uani 1 1 d .
O58 O 1.0823(7) 0.9631(7) -0.0742(5) 0.035(3) Uani 1 1 d .
O59 O 1.2474(6) 1.0994(6) -0.3549(5) 0.027(2) Uani 1 1 d .
O60 O 1.2669(7) 0.5764(7) -0.5189(5) 0.035(3) Uani 1 1 d .
O61 O 1.3405(8) 0.8588(7) 0.0725(5) 0.038(3) Uani 1 1 d .
O62 O 1.4724(6) 0.9457(6) -0.3888(4) 0.027(2) Uani 1 1 d .
O63 O 1.1527(7) 0.9047(8) 0.0453(6) 0.047(3) Uani 1 1 d .
O64 O 0.9327(7) 0.5736(7) -0.4404(5) 0.039(3) Uani 1 1 d .
O65 O 1.1270(7) 0.8328(8) -0.5418(5) 0.038(3) Uani 1 1 d .
O66 O 0.6530(6) 0.7502(6) -0.1389(4) 0.022(2) Uani 1 1 d .
O67 O 0.4771(6) 0.5324(6) -0.3535(5) 0.028(2) Uani 1 1 d .
O68 O 0.9567(6) 0.6057(6) -0.2773(4) 0.020(2) Uani 1 1 d .
O69 O 0.8902(7) 0.7252(7) 0.0249(4) 0.032(2) Uani 1 1 d .
O70 O 1.1145(7) 1.0697(6) -0.2908(5) 0.031(2) Uani 1 1 d .
O71 O 1.2936(6) 0.8956(7) -0.4544(5) 0.029(2) Uani 1 1 d .
O72 O 1.1604(7) 1.1111(7) -0.1572(5) 0.037(3) Uani 1 1 d .
O73 O 1.4348(7) 1.0354(7) 0.0128(5) 0.033(3) Uani 1 1 d .
O74 O 1.1616(7) 0.4209(7) -0.4275(5) 0.040(3) Uani 1 1 d .
O75 O 1.4235(7) 1.1511(6) 0.1015(5) 0.037(3) Uani 1 1 d .
O76 O 0.8877(6) 0.6997(6) -0.3734(5) 0.029(2) Uani 1 1 d .
O77 O 1.2792(8) 0.9170(8) 0.1677(5) 0.048(3) Uani 1 1 d .
O78 O 1.0683(7) 1.0516(7) -0.4253(5) 0.036(3) Uani 1 1 d .
O79 O 1.4115(6) 0.8996(6) -0.2775(4) 0.022(2) Uani 1 1 d .
O80 O 0.5296(7) 0.8382(7) -0.4498(5) 0.041(3) Uani 1 1 d .
O81 O 0.8648(6) 0.6171(6) -0.0874(4) 0.025(2) Uani 1 1 d .
O82 O 0.6242(8) 1.0854(8) -0.3050(6) 0.052(3) Uani 1 1 d .
O83 O 0.5779(8) 0.8880(8) -0.2908(5) 0.044(3) Uani 1 1 d .
O84 O 0.7463(15) 0.5524(10) 0.0329(7) 0.121(8) Uani 1 1 d .
O85 O 1.1566(6) 0.9388(6) -0.4245(5) 0.029(2) Uani 1 1 d .
O86 O 1.3221(7) 0.5304(7) -0.3072(5) 0.038(3) Uani 1 1 d .
O87 O 0.9591(19) 0.585(2) 0.2017(11) 0.179(13) Uani 1 1 d .
O88 O 0.7622(9) 0.5434(8) 0.1685(7) 0.061(4) Uani 1 1 d .
O89 O 1.0025(14) 0.6430(16) 0.0763(11) 0.145(10) Uani 1 1 d .
O90 O 0.7803(10) 0.7132(9) 0.1230(8) 0.075(5) Uani 1 1 d .
O91 O 0.5878(8) 1.0545(8) -0.4575(5) 0.046(3) Uani 1 1 d .
O92 O 0.7045(8) 0.9663(8) -0.4680(6) 0.046(3) Uani 1 1 d .
O93 O 0.7668(9) 1.1077(10) -0.3713(7) 0.080(5) Uani 1 1 d .
O94 O 0.7601(11) 1.0120(10) -0.2693(6) 0.078(5) Uani 1 1 d .
O95 O 1.001(2) 0.789(2) 0.1548(15) 0.077(9) Uiso 0.50 1 d P
O96 O 0.878(3) 0.488(2) 0.121(2) 0.099(13) Uani 0.50 1 d PU
O96' O 0.875(3) 0.511(3) 0.060(2) 0.129(18) Uani 0.50 1 d P
O97 O 0.920(4) 0.733(3) 0.222(2) 0.19(3) Uani 0.50 1 d PU
O101 O 1.0211(17) 0.9196(16) 0.1006(12) 0.149(9) Uiso 1 1 d .
O102 O 1.0974(11) 0.2467(10) -0.4469(10) 0.108(7) Uani 1 1 d .
O103 O 1.3846(12) 1.1633(12) -0.0791(8) 0.110(6) Uani 1 1 d .
O104 O 0.6392(13) 1.2429(10) -0.3473(8) 0.092(5) Uani 1 1 d .
O105 O 0.6185(12) 0.5526(13) 0.2103(9) 0.103(6) Uani 1 1 d .
O106 O 1.2583(11) 0.2100(8) -0.4533(6) 0.075(5) Uani 1 1 d .
O107 O 1.4225(10) 0.8050(11) -0.0135(6) 0.077(5) Uani 1 1 d .
O108 O 0.4200(11) 0.3056(10) -0.1830(9) 0.091(6) Uani 1 1 d .
O109 O 1.4766(11) 0.7142(12) -0.2516(7) 0.087(5) Uani 1 1 d .
O110 O 1.1952(11) 0.7281(10) 0.1669(9) 0.096(6) Uani 1 1 d .
O111 O 0.8618(8) 0.9357(9) -0.4474(6) 0.058(4) Uani 1 1 d .
O112 O 1.3327(10) 0.7549(9) -0.5269(7) 0.067(4) Uani 1 1 d .
O113 O 1.1189(11) 0.4898(10) -0.3043(7) 0.076(4) Uani 1 1 d .
O114 O 1.4152(9) 0.8198(8) 0.1879(7) 0.071(4) Uani 1 1 d .
O115 O 0.9641(10) 0.4219(9) -0.4437(7) 0.068(4) Uani 1 1 d .
O116 O 1.4704(9) 1.3294(9) -0.3583(6) 0.065(4) Uani 1 1 d .
O117 O 1.0951(8) 0.7324(8) -0.0059(6) 0.050(3) Uani 1 1 d .
O118 O 1.5663(7) 0.7049(8) -0.4996(5) 0.045(3) Uani 1 1 d .
O119 O 1.1443(17) 0.7443(13) 0.2836(10) 0.134(8) Uani 1 1 d .
O120 O 0.4721(14) 1.1315(14) -0.4180(10) 0.035(5) Uani 0.50 1 d P
O121 O 0.9314(13) 1.0518(16) -0.2659(14) 0.164(11) Uani 1 1 d .
O122 O 1.2125(19) 1.2658(18) -0.2928(13) 0.065(8) Uiso 0.50 1 d P
O123 O 0.779(5) 0.368(3) -0.017(3) 0.19(3) Uani 0.50 1 d P
O124 O 0.999(3) 1.167(3) -0.341(2) 0.130(15) Uiso 0.50 1 d P
O125 O 1.378(3) 1.321(3) -0.0365(16) 0.17(2) Uani 0.50 1 d PU
O126 O 0.641(5) 0.368(4) -0.0555(19) 0.21(3) Uani 0.50 1 d P
O127 O 1.421(3) 0.626(4) -0.0522(16) 0.139(19) Uani 0.50 1 d P
O128 O 0.796(2) 0.3465(19) 0.031(2) 0.093(13) Uani 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O10 W1 O34 103.7(4) . .
O10 W1 O79 101.8(4) . .
O34 W1 O79 93.2(4) . .
O10 W1 O4 95.9(4) . .
O34 W1 O4 89.9(4) . .
O79 W1 O4 160.8(4) . .
O10 W1 O56 91.1(4) . .
O34 W1 O56 165.2(4) . .
O79 W1 O56 84.9(4) . .
O4 W1 O56 87.3(4) . .
O10 W1 O39 160.8(4) . .
O34 W1 O39 92.5(4) . .
O79 W1 O39 87.2(4) . .
O4 W1 O39 73.7(3) . .
O56 W1 O39 72.8(3) . .
O17 W2 O66 100.2(4) . .
O17 W2 O45 101.0(4) . .
O66 W2 O45 95.7(4) . .
O17 W2 O35 101.7(4) . .
O66 W2 O35 89.6(4) . .
O45 W2 O35 155.3(4) . .
O17 W2 O57 97.9(4) . .
O66 W2 O57 161.5(4) . .
O45 W2 O57 84.5(4) . .
O35 W2 O57 83.0(4) . .
O17 W2 O31 171.6(4) . .
O66 W2 O31 74.4(3) . .
O45 W2 O31 73.5(3) . .
O35 W2 O31 84.9(3) . .
O57 W2 O31 88.0(3) . .
O29 W3 O13 103.6(4) . .
O29 W3 O3 98.8(4) . .
O13 W3 O3 95.1(4) . .
O29 W3 O8 95.1(4) . .
O13 W3 O8 91.5(4) . .
O3 W3 O8 162.7(4) . .
O29 W3 O21 92.5(4) . .
O13 W3 O21 163.6(4) . .
O3 W3 O21 85.7(4) . .
O8 W3 O21 83.4(3) . .
O29 W3 O6 163.3(4) . .
O13 W3 O6 89.5(4) . .
O3 W3 O6 90.2(3) . .
O8 W3 O6 73.8(3) . .
O21 W3 O6 74.1(3) . .
O29 W3 W4 128.5(3) . .
O13 W3 W4 84.7(3) . .
O3 W3 W4 131.5(3) . .
O8 W3 W4 33.3(3) . .
O21 W3 W4 82.5(2) . .
O6 W3 W4 41.3(2) . .
O38 W4 O76 103.7(4) . .
O38 W4 O8 99.3(4) . .
O76 W4 O8 94.4(4) . .
O38 W4 O41 98.9(4) . .
O76 W4 O41 88.4(4) . .
O8 W4 O41 160.4(3) . .
O38 W4 O11 90.9(4) . .
O76 W4 O11 164.6(4) . .
O8 W4 O11 88.2(4) . .
O41 W4 O11 84.3(4) . .
O38 W4 O6 162.9(4) . .
O76 W4 O6 93.0(4) . .
O8 W4 O6 75.1(3) . .
O41 W4 O6 85.4(3) . .
O11 W4 O6 73.0(3) . .
O38 W4 W3 134.0(3) . .
O76 W4 W3 88.5(3) . .
O8 W4 W3 34.9(2) . .
O41 W4 W3 126.0(2) . .
O11 W4 W3 84.9(2) . .
O6 W4 W3 41.0(2) . .
O23 W5 O44 101.4(4) . .
O23 W5 O56 100.7(4) . .
O44 W5 O56 95.7(4) . .
O23 W5 O19 98.3(4) . .
O44 W5 O19 157.7(4) . .
O56 W5 O19 90.7(4) . .
O23 W5 O14 98.3(4) . .
O44 W5 O14 86.5(4) . .
O56 W5 O14 160.0(4) . .
O19 W5 O14 80.4(3) . .
O23 W5 O39 171.7(4) . .
O44 W5 O39 86.8(3) . .
O56 W5 O39 76.5(3) . .
O19 W5 O39 74.0(3) . .
O14 W5 O39 83.8(3) . .
O49 W6 O15 104.0(4) . .
O49 W6 O3 93.7(4) . .
O15 W6 O3 100.0(4) . .
O49 W6 O37 94.4(4) . .
O15 W6 O37 96.2(4) . .
O3 W6 O37 159.6(4) . .
O49 W6 O31 94.7(4) . .
O15 W6 O31 159.9(4) . .
O3 W6 O31 86.1(3) . .
O37 W6 O31 74.6(3) . .
O49 W6 O66 167.6(4) . .
O15 W6 O66 88.3(4) . .
O3 W6 O66 85.6(4) . .
O37 W6 O66 82.5(4) . .
O31 W6 O66 72.9(3) . .
O49 W6 W14 87.6(3) . .
O15 W6 W14 131.0(3) . .
O3 W6 W14 127.1(2) . .
O37 W6 W14 34.8(3) . .
O31 W6 W14 41.2(2) . .
O66 W6 W14 83.0(2) . .
O62 W7 O71 99.9(4) . .
O62 W7 O18 97.8(4) . .
O71 W7 O18 96.2(4) . .
O62 W7 O51 101.7(4) . .
O71 W7 O51 90.1(4) . .
O18 W7 O51 158.1(4) . .
O62 W7 O79 94.9(4) . .
O71 W7 O79 164.6(4) . .
O18 W7 O79 85.6(4) . .
O51 W7 O79 82.9(4) . .
O62 W7 O7 171.6(4) . .
O71 W7 O7 77.1(4) . .
O18 W7 O7 74.9(3) . .
O51 W7 O7 86.2(3) . .
O79 W7 O7 88.7(3) . .
O26 W8 O57 102.9(4) . .
O26 W8 O16 100.6(4) . .
O57 W8 O16 92.9(4) . .
O26 W8 O48 95.0(4) . .
O57 W8 O48 161.3(4) . .
O16 W8 O48 89.0(4) . .
O26 W8 O28 94.7(4) . .
O57 W8 O28 87.5(4) . .
O16 W8 O28 164.2(4) . .
O48 W8 O28 85.7(4) . .
O26 W8 O33 163.3(4) . .
O57 W8 O33 88.2(4) . .
O16 W8 O33 91.1(3) . .
O48 W8 O33 73.2(3) . .
O28 W8 O33 73.1(3) . .
O25 W9 O43 101.4(4) . .
O25 W9 O50 104.1(4) . .
O43 W9 O50 89.8(4) . .
O25 W9 O4 95.4(4) . .
O43 W9 O4 92.0(4) . .
O50 W9 O4 159.6(4) . .
O25 W9 O19 97.2(4) . .
O43 W9 O19 161.3(4) . .
O50 W9 O19 83.7(4) . .
O4 W9 O19 88.2(4) . .
O25 W9 O39 166.2(4) . .
O43 W9 O39 88.2(4) . .
O50 W9 O39 85.5(3) . .
O4 W9 O39 74.3(3) . .
O19 W9 O39 73.8(3) . .
O30 W10 O41 102.4(4) . .
O30 W10 O48 100.0(4) . .
O41 W10 O48 92.7(4) . .
O30 W10 O68 100.7(4) . .
O41 W10 O68 88.6(4) . .
O48 W10 O68 158.4(3) . .
O30 W10 O52 96.5(4) . .
O41 W10 O52 160.3(4) . .
O48 W10 O52 89.3(4) . .
O68 W10 O52 82.5(4) . .
O30 W10 O33 168.8(4) . .
O41 W10 O33 87.7(3) . .
O48 W10 O33 74.2(3) . .
O68 W10 O33 84.3(3) . .
O52 W10 O33 74.1(3) . .
O78 W11 O1 103.5(5) . .
O78 W11 O85 101.7(4) . .
O1 W11 O85 96.4(4) . .
O78 W11 O70 94.8(4) . .
O1 W11 O70 91.1(4) . .
O85 W11 O70 159.7(4) . .
O78 W11 O59 94.2(4) . .
O1 W11 O59 161.5(4) . .
O85 W11 O59 85.4(4) . .
O70 W11 O59 81.6(4) . .
O78 W11 O5 162.6(4) . .
O1 W11 O5 89.1(4) . .
O85 W11 O5 88.4(4) . .
O70 W11 O5 72.8(3) . .
O59 W11 O5 72.4(3) . .
O27 W12 O59 99.0(4) . .
O27 W12 O22 99.5(4) . .
O59 W12 O22 95.9(4) . .
O27 W12 O51 100.0(4) . .
O59 W12 O51 93.0(4) . .
O22 W12 O51 157.0(4) . .
O27 W12 O34 96.1(4) . .
O59 W12 O34 164.8(4) . .
O22 W12 O34 83.3(4) . .
O51 W12 O34 82.6(4) . .
O27 W12 O5 171.9(4) . .
O59 W12 O5 75.9(4) . .
O22 W12 O5 75.0(4) . .
O51 W12 O5 86.7(3) . .
O34 W12 O5 89.3(4) . .
O67 W13 O11 99.5(4) . .
O67 W13 O21 97.4(4) . .
O11 W13 O21 95.0(4) . .
O67 W13 O35 102.1(4) . .
O11 W13 O35 156.7(4) . .
O21 W13 O35 90.6(4) . .
O67 W13 O16 99.2(4) . .
O11 W13 O16 84.7(4) . .
O21 W13 O16 163.2(4) . .
O35 W13 O16 83.5(4) . .
O67 W13 O6 169.0(4) . .
O11 W13 O6 73.6(3) . .
O21 W13 O6 75.1(3) . .
O35 W13 O6 86.1(3) . .
O16 W13 O6 88.8(3) . .
O69 W14 O20 105.4(4) . .
O69 W14 O37 100.6(4) . .
O20 W14 O37 93.9(4) . .
O69 W14 O81 97.4(4) . .
O20 W14 O81 90.3(4) . .
O37 W14 O81 159.7(4) . .
O69 W14 O45 91.0(4) . .
O20 W14 O45 163.5(4) . .
O37 W14 O45 84.8(4) . .
O81 W14 O45 85.6(4) . .
O69 W14 O31 164.4(4) . .
O20 W14 O31 89.8(4) . .
O37 W14 O31 74.7(3) . .
O81 W14 O31 85.5(3) . .
O45 W14 O31 73.9(3) . .
O69 W14 W6 136.0(3) . .
O20 W14 W6 84.4(3) . .
O37 W14 W6 35.4(3) . .
O81 W14 W6 125.9(3) . .
O45 W14 W6 85.1(3) . .
O31 W14 W6 40.8(2) . .
O36 W15 O12 104.9(4) . .
O36 W15 O46 99.0(4) . .
O12 W15 O46 95.0(4) . .
O36 W15 O44 98.4(4) . .
O12 W15 O44 90.0(4) . .
O46 W15 O44 160.0(4) . .
O36 W15 O18 90.5(4) . .
O12 W15 O18 164.5(4) . .
O46 W15 O18 84.4(4) . .
O44 W15 O18 85.6(4) . .
O36 W15 O7 162.3(4) . .
O12 W15 O7 92.2(4) . .
O46 W15 O7 74.2(4) . .
O44 W15 O7 86.2(3) . .
O18 W15 O7 72.7(3) . .
O36 W15 W18 133.3(3) . .
O12 W15 W18 85.8(3) . .
O46 W15 W18 34.3(3) . .
O44 W15 W18 127.4(2) . .
O18 W15 W18 85.0(2) . .
O7 W15 W18 41.7(2) . .
O72 W16 O47 102.7(5) . .
O72 W16 O70 100.6(5) . .
O47 W16 O70 95.8(5) . .
O72 W16 O43 98.1(4) . .
O47 W16 O43 86.0(4) . .
O70 W16 O43 160.3(4) . .
O72 W16 O22 91.8(4) . .
O47 W16 O22 163.5(4) . .
O70 W16 O22 89.1(4) . .
O43 W16 O22 84.2(4) . .
O72 W16 O5 164.0(4) . .
O47 W16 O5 93.2(4) . .
O70 W16 O5 76.1(4) . .
O43 W16 O5 84.2(3) . .
O22 W16 O5 72.6(3) . .
O14 W17 O2 103.4(4) . .
O14 W17 O68 97.2(3) . .
O2 W17 O68 89.3(4) . .
O14 W17 O50 87.9(4) . .
O2 W17 O50 94.5(4) . .
O68 W17 O50 172.8(4) . .
O14 W17 O9 91.4(4) . .
O2 W17 O9 164.2(4) . .
O68 W17 O9 83.1(4) . .
O50 W17 O9 91.7(4) . .
O14 W17 O32 163.6(4) . .
O2 W17 O32 90.0(4) . .
O68 W17 O32 92.5(3) . .
O50 W17 O32 81.4(4) . .
O9 W17 O32 76.6(3) . .
O14 W17 Zn3 128.7(3) . .
O2 W17 Zn3 127.9(3) . .
O68 W17 Zn3 86.8(3) . .
O50 W17 Zn3 86.0(3) . .
O9 W17 Zn3 38.1(2) . .
O32 W17 Zn3 38.5(2) . .
O24 W18 O65 104.1(5) . .
O24 W18 O85 94.1(4) . .
O65 W18 O85 101.1(5) . .
O24 W18 O46 94.2(4) . .
O65 W18 O46 96.6(4) . .
O85 W18 O46 158.0(4) . .
O24 W18 O71 167.1(4) . .
O65 W18 O71 88.6(4) . .
O85 W18 O71 85.7(4) . .
O46 W18 O71 81.7(4) . .
O24 W18 O7 95.2(4) . .
O65 W18 O7 158.9(4) . .
O85 W18 O7 85.7(4) . .
O46 W18 O7 73.3(3) . .
O71 W18 O7 71.9(4) . .
O24 W18 W15 87.1(3) . .
O65 W18 W15 130.8(4) . .
O85 W18 W15 126.1(3) . .
O46 W18 W15 34.3(3) . .
O71 W18 W15 82.6(3) . .
O7 W18 W15 40.8(2) . .
O42 W19 O28 100.8(5) . .
O42 W19 O81 102.0(4) . .
O28 W19 O81 96.0(4) . .
O42 W19 O52 97.5(4) . .
O28 W19 O52 90.5(4) . .
O81 W19 O52 157.8(4) . .
O42 W19 O2 97.5(4) . .
O28 W19 O2 160.7(4) . .
O81 W19 O2 86.0(4) . .
O52 W19 O2 81.2(4) . .
O42 W19 O33 171.9(4) . .
O28 W19 O33 76.0(4) . .
O81 W19 O33 85.8(4) . .
O52 W19 O33 75.2(3) . .
O2 W19 O33 85.1(3) . .
O29 Gd1 O93 99.3(5) . .
O29 Gd1 O91 140.3(3) . .
O93 Gd1 O91 73.8(5) . .
O29 Gd1 O80 74.4(3) . .
O93 Gd1 O80 141.8(4) . .
O91 Gd1 O80 87.3(4) . .
O29 Gd1 O83 75.3(3) . .
O93 Gd1 O83 130.5(4) . .
O91 Gd1 O83 138.9(4) . .
O80 Gd1 O83 85.1(4) . .
O29 Gd1 O82 135.7(4) . .
O93 Gd1 O82 72.4(5) . .
O91 Gd1 O82 80.6(4) . .
O80 Gd1 O82 137.7(4) . .
O83 Gd1 O82 78.3(4) . .
O29 Gd1 O92 69.0(3) . .
O93 Gd1 O92 69.5(4) . .
O91 Gd1 O92 72.1(4) . .
O80 Gd1 O92 73.3(4) . .
O83 Gd1 O92 142.0(4) . .
O82 Gd1 O92 137.8(4) . .
O29 Gd1 O62 130.5(3) . 1_455
O93 Gd1 O62 130.2(5) . 1_455
O91 Gd1 O62 68.5(4) . 1_455
O80 Gd1 O62 67.4(3) . 1_455
O83 Gd1 O62 71.3(3) . 1_455
O82 Gd1 O62 70.4(4) . 1_455
O92 Gd1 O62 124.5(4) . 1_455
O29 Gd1 O94 66.8(4) . .
O93 Gd1 O94 65.5(5) . .
O91 Gd1 O94 135.3(4) . .
O80 Gd1 O94 136.7(4) . .
O83 Gd1 O94 67.5(5) . .
O82 Gd1 O94 70.4(4) . .
O92 Gd1 O94 108.2(4) . .
O62 Gd1 O94 127.3(4) 1_455 .
O54 Gd2 O40 73.4(3) . .
O54 Gd2 O53 94.2(4) . .
O40 Gd2 O53 136.8(3) . .
O54 Gd2 O60 75.6(4) . .
O40 Gd2 O60 79.6(3) . .
O53 Gd2 O60 138.3(3) . .
O54 Gd2 O36 132.1(3) . .
O40 Gd2 O36 70.3(3) . .
O53 Gd2 O36 133.7(3) . .
O60 Gd2 O36 68.0(3) . .
O54 Gd2 O74 140.2(3) . .
O40 Gd2 O74 139.3(3) . .
O53 Gd2 O74 74.5(4) . .
O60 Gd2 O74 87.9(4) . .
O36 Gd2 O74 69.1(3) . .
O54 Gd2 O38 71.2(3) . 2_764
O40 Gd2 O38 136.2(3) . 2_764
O53 Gd2 O38 71.1(3) . 2_764
O60 Gd2 O38 67.3(3) . 2_764
O36 Gd2 O38 118.4(3) . 2_764
O74 Gd2 O38 69.0(3) . 2_764
O54 Gd2 O86 137.2(3) . .
O40 Gd2 O86 83.1(3) . .
O53 Gd2 O86 78.8(4) . .
O60 Gd2 O86 135.1(3) . .
O36 Gd2 O86 67.2(3) . .
O74 Gd2 O86 79.0(4) . .
O38 Gd2 O86 140.7(3) 2_764 .
O54 Gd2 O67 68.7(3) . 1_655
O40 Gd2 O67 69.9(3) . 1_655
O53 Gd2 O67 67.1(3) . 1_655
O60 Gd2 O67 138.0(3) . 1_655
O36 Gd2 O67 123.5(3) . 1_655
O74 Gd2 O67 134.0(4) . 1_655
O38 Gd2 O67 118.1(3) 2_764 1_655
O86 Gd2 O67 69.8(3) . 1_655
O89 Gd3 O90 142.8(5) . .
O89 Gd3 O84 103.8(9) . .
O90 Gd3 O84 78.6(7) . .
O89 Gd3 O96' 57.7(14) . .
O90 Gd3 O96' 139.5(9) . .
O84 Gd3 O96' 61.0(9) . .
O89 Gd3 O88 141.2(6) . .
O90 Gd3 O88 75.5(5) . .
O84 Gd3 O88 73.0(5) . .
O96' Gd3 O88 90.0(14) . .
O89 Gd3 O87 77.1(6) . .
O90 Gd3 O87 131.2(6) . .
O84 Gd3 O87 127.5(9) . .
O96' Gd3 O87 78.3(11) . .
O88 Gd3 O87 75.5(7) . .
O89 Gd3 O97 114.5(15) . .
O90 Gd3 O97 66.9(10) . .
O84 Gd3 O97 141.0(13) . .
O96' Gd3 O97 148.8(13) . .
O88 Gd3 O97 81.1(16) . .
O87 Gd3 O97 70.5(11) . .
O89 Gd3 O69 69.7(4) . .
O90 Gd3 O69 75.6(4) . .
O84 Gd3 O69 74.3(4) . .
O96' Gd3 O69 94.2(13) . .
O88 Gd3 O69 139.8(4) . .
O87 Gd3 O69 144.4(6) . .
O97 Gd3 O69 111.9(14) . .
O89 Gd3 O95 73.5(10) . .
O90 Gd3 O95 83.0(8) . .
O84 Gd3 O95 143.5(8) . .
O96' Gd3 O95 131.0(14) . .
O88 Gd3 O95 131.8(8) . .
O87 Gd3 O95 88.1(11) . .
O97 Gd3 O95 50.8(16) . .
O69 Gd3 O95 70.6(8) . .
O89 Gd3 O96 73.1(8) . .
O90 Gd3 O96 141.5(8) . .
O84 Gd3 O96 78.5(12) . .
O96' Gd3 O96 32.2(12) . .
O88 Gd3 O96 68.4(7) . .
O87 Gd3 O96 51.0(12) . .
O97 Gd3 O96 118.4(16) . .
O69 Gd3 O96 126.2(9) . .
O95 Gd3 O96 131.7(12) . .
O73 Gd4 O15 137.3(3) . 2_775
O73 Gd4 O75 69.2(3) . .
O15 Gd4 O75 71.0(3) 2_775 .
O73 Gd4 O61 82.0(4) . .
O15 Gd4 O61 139.1(3) 2_775 .
O75 Gd4 O61 134.6(3) . .
O73 Gd4 O77 141.0(4) . .
O15 Gd4 O77 71.9(3) 2_775 .
O75 Gd4 O77 115.4(4) . .
O61 Gd4 O77 68.0(4) . .
O73 Gd4 O63 132.7(3) . .
O15 Gd4 O63 73.1(3) 2_775 .
O75 Gd4 O63 138.0(4) . .
O61 Gd4 O63 87.3(4) . .
O77 Gd4 O63 72.0(4) . .
O73 Gd4 O55 80.9(3) . .
O15 Gd4 O55 72.7(3) 2_775 .
O75 Gd4 O55 72.0(3) . .
O61 Gd4 O55 138.1(3) . .
O77 Gd4 O55 138.2(4) . .
O63 Gd4 O55 77.1(4) . .
O73 Gd4 O25 68.6(3) . .
O15 Gd4 O25 128.1(3) 2_775 .
O75 Gd4 O25 126.3(3) . .
O61 Gd4 O25 68.3(3) . .
O77 Gd4 O25 118.3(3) . .
O63 Gd4 O25 64.6(3) . .
O55 Gd4 O25 69.8(3) . .
O73 Gd4 O10 76.7(3) . 2_875
O15 Gd4 O10 102.3(3) 2_775 2_875
O75 Gd4 O10 68.1(3) . 2_875
O61 Gd4 O10 71.7(3) . 2_875
O77 Gd4 O10 70.7(4) . 2_875
O63 Gd4 O10 141.8(4) . 2_875
O55 Gd4 O10 139.0(3) . 2_875
O25 Gd4 O10 129.6(3) . 2_875
O31 Zn1 O6 107.8(3) . .
O31 Zn1 O33 108.1(4) . .
O6 Zn1 O33 102.4(4) . .
O31 Zn1 O32 109.4(4) . .
O6 Zn1 O32 113.6(4) . .
O33 Zn1 O32 115.1(4) . .
O5 Zn2 O7 107.6(4) . .
O5 Zn2 O39 103.5(4) . .
O7 Zn2 O39 106.8(4) . .
O5 Zn2 O9 115.1(4) . .
O7 Zn2 O9 109.8(3) . .
O39 Zn2 O9 113.5(4) . .
O13 Zn3 O1 94.5(4) . .
O13 Zn3 O9 164.0(4) . .
O1 Zn3 O9 95.7(4) . .
O13 Zn3 O32 95.1(4) . .
O1 Zn3 O32 164.5(4) . .
O9 Zn3 O32 77.8(3) . .
O13 Zn3 O76 88.8(3) . .
O1 Zn3 O76 96.5(4) . .
O9 Zn3 O76 77.8(3) . .
O32 Zn3 O76 95.8(3) . .
O13 Zn3 O47 97.0(3) . .
O1 Zn3 O47 89.1(4) . .
O9 Zn3 O47 95.6(3) . .
O32 Zn3 O47 77.7(3) . .
O76 Zn3 O47 171.7(4) . .
O13 Zn3 W17 132.5(3) . .
O1 Zn3 W17 133.0(3) . .
O9 Zn3 W17 38.7(2) . .
O32 Zn3 W17 39.1(2) . .
O76 Zn3 W17 85.5(3) . .
O47 Zn3 W17 86.1(2) . .
O20 Cu1 O32 94.0(4) . .
O20 Cu1 O47 177.2(4) . .
O32 Cu1 O47 86.8(4) . .
O20 Cu1 O58 86.5(4) . .
O32 Cu1 O58 172.0(4) . .
O47 Cu1 O58 92.4(4) . .
O20 Cu1 O49 89.2(4) . .
O32 Cu1 O49 97.2(3) . .
O47 Cu1 O49 93.3(4) . .
O58 Cu1 O49 90.8(4) . .
O20 Cu1 O50 95.4(4) . .
O32 Cu1 O50 72.6(3) . .
O47 Cu1 O50 82.3(4) . .
O58 Cu1 O50 99.4(4) . .
O49 Cu1 O50 169.0(3) . .
O64 Cu2 O12 87.3(4) . .
O64 Cu2 O76 93.6(4) . .
O12 Cu2 O76 175.9(4) . .
O64 Cu2 O9 172.8(4) . .
O12 Cu2 O9 93.1(4) . .
O76 Cu2 O9 85.6(4) . .
O64 Cu2 O24 90.8(4) . .
O12 Cu2 O24 91.5(4) . .
O76 Cu2 O24 92.5(4) . .
O9 Cu2 O24 96.4(4) . .
O64 Cu2 O68 101.0(4) . .
O12 Cu2 O68 93.9(3) . .
O76 Cu2 O68 82.0(4) . .
O9 Cu2 O68 71.9(3) . .
O24 Cu2 O68 167.3(3) . .
W11 O1 Zn3 144.2(5) . .
W17 O2 W19 144.2(5) . .
W3 O3 W6 148.2(5) . .
W9 O4 W1 113.6(4) . .
Zn2 O5 W16 121.2(4) . .
Zn2 O5 W11 113.9(4) . .
W16 O5 W11 97.0(3) . .
Zn2 O5 W12 123.6(4) . .
W16 O5 W12 98.0(3) . .
W11 O5 W12 97.8(4) . .
Zn1 O6 W3 114.5(4) . .
Zn1 O6 W4 121.9(4) . .
W3 O6 W4 97.6(3) . .
Zn1 O6 W13 122.0(4) . .
W3 O6 W13 97.8(3) . .
W4 O6 W13 97.8(3) . .
Zn2 O7 W15 116.9(4) . .
Zn2 O7 W18 117.9(4) . .
W15 O7 W18 97.5(3) . .
Zn2 O7 W7 121.5(4) . .
W15 O7 W7 99.2(3) . .
W18 O7 W7 99.3(4) . .
W4 O8 W3 111.7(4) . .
Zn2 O9 Zn3 112.5(4) . .
Zn2 O9 Cu2 116.6(4) . .
Zn3 O9 Cu2 101.9(4) . .
Zn2 O9 W17 114.7(4) . .
Zn3 O9 W17 103.1(4) . .
Cu2 O9 W17 106.6(4) . .
W1 O10 Gd4 156.5(5) . 2_875
W13 O11 W4 115.4(4) . .
W15 O12 Cu2 138.8(6) . .
W3 O13 Zn3 143.4(5) . .
W17 O14 W5 146.7(5) . .
W6 O15 Gd4 156.7(5) . 2_775
W8 O16 W13 145.1(5) . .
W7 O18 W15 113.2(4) . .
W5 O19 W9 113.5(4) . .
W14 O20 Cu1 140.9(5) . .
W13 O21 W3 113.0(4) . .
W12 O22 W16 113.9(5) . .
W18 O24 Cu2 131.6(5) . .
W9 O25 Gd4 156.8(5) . .
W19 O28 W8 112.8(5) . .
W3 O29 Gd1 156.7(5) . .
Zn1 O31 W6 120.7(4) . .
Zn1 O31 W14 117.1(4) . .
W6 O31 W14 98.0(3) . .
Zn1 O31 W2 120.1(4) . .
W6 O31 W2 98.6(3) . .
W14 O31 W2 97.6(3) . .
Zn1 O32 Cu1 116.5(4) . .
Zn1 O32 Zn3 113.4(4) . .
Cu1 O32 Zn3 101.8(4) . .
Zn1 O32 W17 113.7(4) . .
Cu1 O32 W17 107.5(4) . .
Zn3 O32 W17 102.4(4) . .
Zn1 O33 W8 124.3(4) . .
Zn1 O33 W19 115.5(4) . .
W8 O33 W19 97.8(4) . .
Zn1 O33 W10 118.3(4) . .
W8 O33 W10 98.2(4) . .
W19 O33 W10 97.7(3) . .
W1 O34 W12 144.3(5) . .
W13 O35 W2 160.3(5) . .
W15 O36 Gd2 161.3(5) . .
W14 O37 W6 109.8(4) . .
W4 O38 Gd2 157.2(5) . 2_764
Zn2 O39 W9 117.4(4) . .
Zn2 O39 W1 123.1(4) . .
W9 O39 W1 97.9(3) . .
Zn2 O39 W5 117.0(4) . .
W9 O39 W5 98.7(4) . .
W1 O39 W5 98.1(3) . .
W10 O41 W4 153.4(5) . .
W9 O43 W16 154.1(5) . .
W5 O44 W15 160.0(5) . .
W2 O45 W14 114.9(5) . .
W15 O46 W18 111.4(4) . .
W16 O47 Cu1 136.9(5) . .
W16 O47 Zn3 129.2(5) . .
Cu1 O47 Zn3 91.1(4) . .
W10 O48 W8 114.0(4) . .
W6 O49 Cu1 131.3(5) . .
W9 O50 W17 143.1(5) . .
W9 O50 Cu1 119.2(4) . .
W17 O50 Cu1 96.5(3) . .
W12 O51 W7 160.1(5) . .
W19 O52 W10 113.0(4) . .
W5 O56 W1 112.5(4) . .
W8 O57 W2 148.9(6) . .
W12 O59 W11 113.6(4) . .
W7 O62 Gd1 156.3(5) . 1_655
W2 O66 W6 114.1(4) . .
W13 O67 Gd2 151.9(5) . 1_455
W17 O68 W10 143.7(5) . .
W17 O68 Cu2 96.2(3) . .
W10 O68 Cu2 119.2(4) . .
W14 O69 Gd3 148.7(6) . .
W16 O70 W11 112.1(4) . .
W7 O71 W18 111.7(5) . .
W4 O76 Cu2 134.8(5) . .
W4 O76 Zn3 129.7(5) . .
Cu2 O76 Zn3 92.1(3) . .
W1 O79 W7 147.9(5) . .
W19 O81 W14 161.4(5) . .
W11 O85 W18 147.5(5) . .
O96' O96 Gd3 69.6(19) . .
O96 O96' Gd3 78(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O10 1.735(9) .
W1 O34 1.839(9) .
W1 O79 1.860(8) .
W1 O4 1.947(9) .
W1 O56 2.073(9) .
W1 O39 2.170(8) .
W2 O17 1.718(9) .
W2 O66 1.842(9) .
W2 O45 1.890(9) .
W2 O35 1.925(9) .
W2 O57 2.001(9) .
W2 O31 2.285(8) .
W3 O29 1.739(9) .
W3 O13 1.794(9) .
W3 O3 1.916(8) .
W3 O8 1.981(8) .
W3 O21 2.082(9) .
W3 O6 2.129(8) .
W3 W4 3.2135(7) .
W4 O38 1.739(9) .
W4 O76 1.801(9) .
W4 O8 1.901(9) .
W4 O41 1.993(9) .
W4 O11 2.048(9) .
W4 O6 2.141(8) .
W5 O23 1.716(9) .
W5 O44 1.870(9) .
W5 O56 1.871(9) .
W5 O19 1.938(8) .
W5 O14 2.048(8) .
W5 O39 2.175(9) .
W6 O49 1.750(9) .
W6 O15 1.771(9) .
W6 O3 1.928(8) .
W6 O37 1.971(9) .
W6 O31 2.114(8) .
W6 O66 2.129(9) .
W6 W14 3.2031(8) .
W7 O62 1.727(9) .
W7 O71 1.857(10) .
W7 O18 1.875(8) .
W7 O51 1.925(8) .
W7 O79 2.014(8) .
W7 O7 2.200(9) .
W8 O26 1.719(10) .
W8 O57 1.843(8) .
W8 O16 1.856(9) .
W8 O48 1.994(8) .
W8 O28 2.043(10) .
W8 O33 2.142(9) .
W9 O25 1.729(8) .
W9 O43 1.853(9) .
W9 O50 1.923(9) .
W9 O4 1.942(9) .
W9 O19 1.982(8) .
W9 O39 2.147(8) .
W10 O30 1.711(9) .
W10 O41 1.871(9) .
W10 O48 1.897(10) .
W10 O68 1.972(9) .
W10 O52 1.991(9) .
W10 O33 2.174(8) .
W11 O78 1.710(10) .
W11 O1 1.783(10) .
W11 O85 1.874(9) .
W11 O70 2.040(9) .
W11 O59 2.077(9) .
W11 O5 2.176(9) .
W12 O27 1.739(10) .
W12 O59 1.862(9) .
W12 O22 1.878(9) .
W12 O51 1.915(8) .
W12 O34 2.076(10) .
W12 O5 2.200(9) .
W13 O67 1.725(9) .
W13 O11 1.872(8) .
W13 O21 1.879(9) .
W13 O35 1.911(9) .
W13 O16 2.026(9) .
W13 O6 2.255(8) .
W14 O69 1.752(9) .
W14 O20 1.775(9) .
W14 O37 1.944(9) .
W14 O81 1.962(9) .
W14 O45 2.053(9) .
W14 O31 2.131(8) .
W15 O36 1.735(8) .
W15 O12 1.761(9) .
W15 O46 1.957(9) .
W15 O44 1.960(9) .
W15 O18 2.074(9) .
W15 O7 2.130(8) .
W15 W18 3.2327(8) .
W16 O72 1.717(9) .
W16 O47 1.783(10) .
W16 O70 1.879(10) .
W16 O43 1.999(9) .
W16 O22 2.050(10) .
W16 O5 2.165(8) .
W17 O14 1.799(8) .
W17 O2 1.846(9) .
W17 O68 1.917(9) .
W17 O50 1.970(9) .
W17 O9 2.033(9) .
W17 O32 2.044(8) .
W17 Zn3 3.1644(15) .
W18 O24 1.734(10) .
W18 O65 1.741(10) .
W18 O85 1.938(9) .
W18 O46 1.957(9) .
W18 O71 2.161(9) .
W18 O7 2.169(9) .
W19 O42 1.706(9) .
W19 O28 1.859(9) .
W19 O81 1.864(9) .
W19 O52 1.932(9) .
W19 O2 2.021(9) .
W19 O33 2.173(9) .
Gd1 O29 2.368(9) .
Gd1 O93 2.407(13) .
Gd1 O91 2.411(11) .
Gd1 O80 2.437(10) .
Gd1 O83 2.440(11) .
Gd1 O82 2.461(11) .
Gd1 O92 2.462(11) .
Gd1 O62 2.467(9) 1_455
Gd1 O94 2.603(14) .
Gd2 O54 2.385(9) .
Gd2 O40 2.391(9) .
Gd2 O53 2.432(10) .
Gd2 O60 2.434(10) .
Gd2 O36 2.461(8) .
Gd2 O74 2.463(10) .
Gd2 O38 2.472(8) 2_764
Gd2 O86 2.482(10) .
Gd2 O67 2.577(9) 1_655
Gd3 O89 2.375(16) .
Gd3 O90 2.387(13) .
Gd3 O84 2.389(17) .
Gd3 O96' 2.40(4) .
Gd3 O88 2.397(12) .
Gd3 O87 2.409(17) .
Gd3 O97 2.46(4) .
Gd3 O69 2.476(10) .
Gd3 O95 2.49(3) .
Gd3 O96 2.50(3) .
Gd4 O73 2.394(10) .
Gd4 O15 2.406(8) 2_775
Gd4 O75 2.416(10) .
Gd4 O61 2.431(10) .
Gd4 O77 2.470(11) .
Gd4 O63 2.488(11) .
Gd4 O55 2.511(10) .
Gd4 O25 2.521(8) .
Gd4 O10 2.537(9) 2_875
Zn1 O31 1.925(8) .
Zn1 O6 1.933(8) .
Zn1 O33 1.944(9) .
Zn1 O32 1.948(9) .
Zn2 O5 1.919(9) .
Zn2 O7 1.932(8) .
Zn2 O39 1.949(9) .
Zn2 O9 1.958(9) .
Zn3 O13 1.950(9) .
Zn3 O1 1.959(10) .
Zn3 O9 2.007(9) .
Zn3 O32 2.015(9) .
Zn3 O76 2.322(9) .
Zn3 O47 2.349(10) .
Cu1 O20 1.982(10) .
Cu1 O32 2.001(8) .
Cu1 O47 2.003(10) .
Cu1 O58 2.021(9) .
Cu1 O49 2.223(9) .
Cu1 O50 2.389(9) .
Cu2 O64 1.976(9) .
Cu2 O12 1.982(9) .
Cu2 O76 2.004(10) .
Cu2 O9 2.014(8) .
Cu2 O24 2.224(11) .
Cu2 O68 2.417(9) .
O10 Gd4 2.537(9) 2_875
O15 Gd4 2.406(8) 2_775
O38 Gd2 2.472(8) 2_764
O62 Gd1 2.467(9) 1_655
O67 Gd2 2.577(9) 1_455
O96 O96' 1.36(5) .
O123 O128 1.11(6) .
